eps){width="9cm"}

In the insulating regime (x$>$0.175), the up-shift of $T_S$ induced by oxygen isotope exchange can be explained to originate from that substitution of $^{16}O$ by $^{18}O$ leads to a decrease in frequency of phonon, and consequently enhances effective mass of electron ($m^*$) through strong electron-phonon coupling. The enhancement of $m^*$ leads to a decrease of bandwidth W, resulting in an increase of energy difference $\Delta E$ between IS and LS states and consequently an up-shift of $T_s$. The increase of Sm-doping leads to a decrease in the ionic radius of A site $(Pr_{1-x}Sm_x)_{0.7}Ca_{0.3}$ in the $(Pr_{1-x}Sm_x)_{0.7}Ca_{0.3}CoO_3$ system, so that volume of the $CoO_6$ octahedra decreases. The decrease in volume of the $CoO_6$ octahedra results in an increase of crystal field splitting energy $\Delta_C$ and $\Delta E$, causing an increase in $T_S$. Therefore, decrease of the isotope component $\alpha_s$ with increasing x could be due to the increase of $T_s$. In contrast to the giant oxygen isotope effect in the insulating phase, a negligible oxygen isotope effect on $T_c$ is observed in the ferromagnetic metal regime. It has been reported that substitution of $^{16}O$ by $^{18}O$ leads to a giant down-shift of Curie temperature in $La_{1-x}Ca_xMnO_{3+y}$.[@zhao] Such giant oxygen isotope shift was explained by the JT polaron formed due to strong Jahn-Teller effect.[@zhao] Recently, elastic and inelastic neutron scattering showed that spin activation of $Co^{+3}$ ions in perovskite cobalt oxides induces local static JT distortions in the insulating phase, while the static JT distortions are absent in the ferromagnetic metal phase.[@louca1] This observation explained that the giant oxygen isotope effect is observed in the insulating phase, while negligible in the ferromagnetic metal phase well. The lattice distortions from the JT effect with strong electron-phonon coupling should be responsible for the giant isotope effect in the insulating phase.

In conclusion, oxygen isotope effect is systematically studied
eps){width="9 cm " } 

 In the insulating regime (x$>$0.175), the up - shift of $ T_S$ induced by oxygen isotope substitution can be excuse to originate from that substitution of $ ^{16}O$ by $ ^{18}O$ leads to a decrease in frequency of phonon, and consequently enhances effective mass of electron ($ m^*$) through potent electron - phonon coupling. The enhancement of $ m^*$ leads to a decrease of bandwidth W, result in an increase of energy deviation $ \Delta E$ between IS and LS states and consequently an up - shift key of $ T_s$. The increase of Sm - doping moderate to a decrease in the ionic spoke of A site $ (Pr_{1 - x}Sm_x)_{0.7}Ca_{0.3}$ in the $ (Pr_{1 - x}Sm_x)_{0.7}Ca_{0.3}CoO_3 $ system, so that bulk of the $ CoO_6 $ octahedra decreases. The decrease in volume of the $ CoO_6 $ octahedra consequence in an increase of crystal field separate energy $ \Delta_C$ and $ \Delta E$, causing an increase in $ T_S$. Therefore, decrease of the isotope component $ \alpha_s$ with increase x could be due to the increase of $ T_s$. In contrast to the giant oxygen isotope effect in the insulate phase, a negligible oxygen isotope effect on $ T_c$ is observed in the ferromagnetic metal regime. It has been reported that substitution of $ ^{16}O$ by $ ^{18}O$ leads to a giant down - shift of Curie temperature in $ La_{1 - x}Ca_xMnO_{3+y}$.[@zhao ] Such giant oxygen isotope shift was explained by the JT polaron formed due to strong Jahn - Teller effect.[@zhao ] Recently, elastic and inelastic neutron scattering showed that spin activation of $ Co^{+3}$ ion in perovskite cobalt oxide induces local static JT distortions in the insulate phase, while the static JT distortions are absent in the ferromagnetic metallic element phase.[@louca1 ] This observation explained that the giant oxygen isotope effect is watch in the insulating phase, while negligible in the ferromagnetic metal phase well. The lattice distortions from the JT effect with strong electron - phonon yoke should be responsible for the giant isotope effect in the insulating phase. 

 In conclusion, oxygen isotope effect is systematically studied
eps){aidth="9cm"}

In the insulating regime (x$>$0.175), the uk-syift oh $T_S$ insuced by oxygen isotope exchange can bw expoained to originate frum that slbstitutiin oh $^{16}O$ by $^{18}O$ leads to a decrccse ih frexnency of phonon, and consexuently enhancas eyfective mass of electron ($m^*$) through ftrong rlfctron-phonon cjuplpnd. Ths enhancement of $m^*$ leads to a decrsase of bandwidth W, tesulting in an increase ov enfrgy difference $\Depta E$ betwegh IF and LS statds and consequently an up-shift of $T_s$. The increase of Rm-dopnng leads ti q dfwrease in tie ionpc radius of A site $(Ps_{1-x}Sm_x)_{0.7}Ca_{0.3}$ in the $(Pr_{1-x}Sm_x)_{0.7}Ga_{0.3}CoO_3$ sywtem, so that volume oh the $CoO_6$ octahedra qecreases. Tke decrease in volume od the $CoO_6$ octxyedfa dexumts in an increase kf crystal dield splitting enetgr $\Delta_C$ and $\Dslta E$, cwusing an increase in $T_S$. Therefore, decrtase kf the isotope componenr $\alpha_s$ with increaslng x coujd be due to the increase of $T_s$. In contrast to tha giait oxvncn iritlpe effect in the insulating phase, a negligibjs pxjgen isotope effegt on $T_c$ is observrd im the ferromagvetic metzl regime. It has bfen repjrted that subftitition of $^{16}O$ by $^{18}O$ leads to a tiant down-shpft if Curie temperatuxe in $La_{1-x}Ca_xOnO_{3+y}$.[@ehao] Sich giant oxygen isotopz shiff was explalned by tgd JT polaron foroed dge to strong Jahn-Teller efsect.[@zhao] Cecencly, elasgic snd inqlastic nektron scattering showed hhat dphn activatlon of $Co^{+3}$ ions in perovskite couelt oxides incuwes local scatic MT distortions yn the insulatnng phasz, whild the statpc JT disvortions are absent in tha ferromagnetmc metal [hasw.[@louxa1] This ubservation exllained tkct the giqnt oxygen isotope efwsct is observed in the insulating phxse, wjike tegligible it thd fdtromaenetic metao phaxe well. The lattice gistkrtions from the JY cffect wijh strong electron-phonpn coupling should be rxsponsmble fpr jhe giant isotope effect in the insulatijg ihase.

In concltsiok, oxigen isotopz effect is systematically studied
eps){width="9cm"} In the insulating regime (x$>$0.175), the $T_S$ by oxygen exchange can be substitution $^{16}O$ by $^{18}O$ to a decrease frequency of phonon, and consequently enhances mass of electron ($m^*$) through strong electron-phonon coupling. The enhancement of $m^*$ leads a decrease of bandwidth W, resulting in an increase of energy difference $\Delta between and states consequently an up-shift of $T_s$. The increase of Sm-doping leads to a decrease in the ionic of A site $(Pr_{1-x}Sm_x)_{0.7}Ca_{0.3}$ in the $(Pr_{1-x}Sm_x)_{0.7}Ca_{0.3}CoO_3$ system, that volume of the octahedra decreases. The decrease in of $CoO_6$ octahedra in increase crystal field splitting $\Delta_C$ and $\Delta E$, causing an increase in $T_S$. Therefore, decrease of the isotope component $\alpha_s$ with x could to the of In to the giant effect in the insulating phase, a effect on $T_c$ is observed in the ferromagnetic regime. It been reported that substitution of $^{16}O$ $^{18}O$ leads to a giant down-shift of Curie in $La_{1-x}Ca_xMnO_{3+y}$.[@zhao] Such giant oxygen isotope shift was explained by the JT polaron formed due Jahn-Teller effect.[@zhao] Recently, elastic inelastic neutron scattering that activation $Co^{+3}$ in perovskite oxides induces local static JT distortions in the insulating phase, while static JT distortions are absent in the ferromagnetic metal phase.[@louca1] explained the giant oxygen effect is observed in insulating while negligible in the phase The the effect strong electron-phonon coupling should responsible for the giant isotope in the insulating phase. is systematically studied
eps){width="9cm"}

In the insulating Regime (x$>$0.175), the Up-shiFt oF $T_S$ InDuceD by oXygen isotope exCHangE can be explained to origiNate fRoM That SUbStituTion of $^{16}O$ BY $^{18}O$ LEAds To A dEcrEaSE iN freqUenCy of phoNon, and consEquEnTly enhances eFFeCtive mass oF elEctron ($m^*$) throuGh sTrong eLeCtrON-phonOn cOupliNg. The eNHancemEnt of $m^*$ leaDs TO a decrEAse of baNDWiDth W, Resulting in an incrEAsE Of energy differEnce $\DeLtA e$ bETWeeN IS And LS stateS aNd conSEquentlY An UP-SHifT Of $T_s$. The increaSe of Sm-dopinG LeaDs to a dEcReaSE in the Ionic RaDIus Of A site $(Pr_{1-x}SM_x)_{0.7}Ca_{0.3}$ In the $(Pr_{1-x}SM_x)_{0.7}Ca_{0.3}Coo_3$ System, sO That volUme of tHe $COO_6$ oCtahEDrA dEcrEaSEs. THE dEcrEAse In volume Of ThE $CoO_6$ oCtahEDRA ResuLts In an IncreAse of crystal fIelD splITtiNg eneRgy $\DeLta_C$ AnD $\DeltA E$, causIng an InCrease in $T_S$. ThereFore, Decrease oF thE iSotOpE compONent $\alPha_S$ wiTh increAsing x cOUld Be DUE To The increase of $T_s$. In cOnTRAsT to the giAnt oxyGEn IsOTope effeCt In tHe inSULatinG phaSE, a NegligibLe oxygEN iSoTope effEcT on $T_c$ iS oBseRveD in thE FerrOmagneTic metal RegimE. it has been reporTEd that substitUTiON Of $^{16}o$ By $^{18}O$ lEadS to a giant doWn-shIFt of curiE TeMpeRAture In $La_{1-x}ca_Xmno_{3+Y}$.[@zhao] Such giant oxygeN iSotope Shift Was explained bY the JT polaRON Formed duE to sTRoNG Jahn-Teller effEct.[@zhAo] Recently, ELastic anD inelAstic neuTron scattERIng showeD thAt sPin ActIVAtIon of $Co^{+3}$ ions in PERovsKiTe cobalT oxIdes indUceS loCal StaTiC JT distorTions in tHe InSuLaTinG phasE, While the StAtiC Jt diStortIOns are AbsenT in tHe FeRRomAgnetic MEtAL PhasE.[@lOuCa1] ThIs oBsErvatIon eXPlaIned thaT the giant OxyGEn isOtOpE effect Is observed in tHe Insulating PhAse, While nEGLigible iN the ferromagnetic metal pHAse well. the LattiCe diStortions FroM the JT EffECt with Strong ElectRoN-phONOn couPLInG shOuLd be responSIBle For thE gIant Isotope Effect in the insulatINg pHase.

In conclusIon, OxygEN IsOtoPE eFFecT iS SysTEMatically studieD
eps){width="9cm"}

In theinsulating  regi me(x$ >$ 0.17 5),the up-shift o f  $T_ S$ induced by oxygen i sotop ee xcha n ge  canbe expl a in e d  to  o ri gin at e  f rom t hat  substi tution of$^{ 16 }O$ by $^{18 } O$  leads toa d ecrease in f req uencyof  ph o non,and  cons equent l y enha nces effe ct i ve mas s  of ele c t ro n ($ m^*$) through str o ng electron-phono n coup li n g. T heenh ancement o f$m^*$ leads t o  a d e cre a se of bandwid th W, resul t ing  in an  i ncr e ase of  ener gy dif ference $\D elta  E$ betwe en ISa nd LS s t ates an d cons equ ent ly a n  u p- shi ft of$ T_ s$. The  increas eof  Sm-d opin g l e adstoa de creas e in the ioni c r adiu s  of  A si te $( Pr_{ 1- x}Sm_ x)_{0. 7}Ca_ {0 .3}$ in the $(P r_{1 -x}Sm_x)_ {0. 7} Ca_ {0 .3}Co O _3$ sy ste m,so that  volume ofth e $ Co O_6$ octahedra dec re a s es . The de crease in  v o lume ofth e $ CoO_ 6 $  octa hedr a  r esults i n an i n cr ea se of c ry stal f ie ldspl ittin g  ene rgy $\ Delta_C$  and$ \Delta E$, cau s ing an increa s ei n  $ T _S$.  Th erefore, de crea s e of  the is oto p e com ponen t$ \a l pha_s$ with increas in g x co uld b e due to theincrease o f $ T_s$. In  con t ra s t to the giant  oxyg en isotope effect i n the  insulat ing phase , a neglig ibl e o xyg eni s ot ope effect on $ T_c$  i s obser ved  in the  fe rro mag net ic  metal re gime. It  h as  b ee n r eport e d that s ub sti tu tio n of$ ^{16}O $ by$^{1 8} O$ lea ds to a gi a n t do wn -s hift  of  C urietemp e rat ure in$La_{1-x} Ca_ x MnO_ {3 +y }$.[@zh ao] Such gian toxygen iso to peshiftw a s explai ned by the JT polaron f o rmed du e t o str ongJahn-Tell ereffect .[@ z hao] R ecentl y, el as tic a nd in e l as tic  n eutron sca t t eri ng sh ow ed t hat spi n activation of $C o ^{+ 3}$ ions in p ero vski t e  c oba l to xid es ind u c es local static  JT distor ti o ns  in the in s ula ti ng phas e, whil e the staticJT distor tions are  a bsen t inthe ferrom agneticmetal pha s e.[@l o uc a1] T his  obser va tio n exp lained tha t the  giant  o xygenisoto pe  effectis observed in the insu lating  phas e,while neg lig i ble  in the f erro magnetic m eta l p hasewel l . The  lat t ic e d i stort ions from theJ Teff e c twith strong e l ect ron-p hon o n coup ling  should be respon s ible for the g iant i sot ope effe ct  in the insula tin gp h ase.

In  c onclusion,oxygen i so t ope e ffectis sys tematic a l ly studie d
eps){width="9cm"}

In the_insulating regime_(x$>$0.175), the up-shift of_$T_S$ induced_by_oxygen isotope_exchange_can be explained_to originate from_that substitution of $^{16}O$_by $^{18}O$ leads_to_a decrease in frequency of phonon, and consequently enhances effective mass of electron ($m^*$)_through_strong electron-phonon_coupling._The_enhancement of $m^*$ leads to_a decrease of bandwidth W,_resulting in_an increase of energy difference $\Delta E$ between_IS_and LS states_and consequently an up-shift of $T_s$. The increase of_Sm-doping leads to a decrease in_the ionic radius_of_A_site $(Pr_{1-x}Sm_x)_{0.7}Ca_{0.3}$ in the_$(Pr_{1-x}Sm_x)_{0.7}Ca_{0.3}CoO_3$ system, so that volume of_the $CoO_6$ octahedra decreases. The decrease_in volume of the $CoO_6$ octahedra results_in an increase of crystal field_splitting energy $\Delta_C$ and $\Delta_E$, causing_an increase in $T_S$. Therefore,_decrease of the_isotope component_$\alpha_s$ with increasing_x could be due to the_increase of $T_s$._In contrast to the giant oxygen_isotope_effect in the_insulating_phase,_a negligible_oxygen isotope effect_on_$T_c$ is_observed_in the ferromagnetic metal regime. It_has_been reported that substitution of $^{16}O$ by_$^{18}O$ leads to a_giant_down-shift of Curie temperature_in $La_{1-x}Ca_xMnO_{3+y}$.[@zhao] Such giant oxygen_isotope shift was explained by the_JT polaron_formed due_to strong Jahn-Teller effect.[@zhao] Recently, elastic and inelastic neutron scattering showed_that spin activation of $Co^{+3}$ ions_in perovskite cobalt oxides_induces local_static_JT distortions in_the_insulating phase,_while the static JT distortions are absent_in the_ferromagnetic metal phase.[@louca1] This observation explained_that the giant oxygen_isotope_effect is observed in the insulating_phase, while negligible in the ferromagnetic_metal phase well. The lattice_distortions_from_the JT effect with strong_electron-phonon coupling should be responsible for_the giant isotope_effect in the insulating phase.

In conclusion, oxygen_isotope_effect is systematically studied